Advanced Optimization Techniques and Their Applications in Civil Engineering
View this Special IssueResearch Article  Open Access
Nitza M. García, Hildélix L. SotoToro, Mauricio CabreraRíos, Oscar Marcelo Suárez, "Optimal Cement Mixtures Containing Mineral Admixtures under Multiple and Conflicting Criteria", Advances in Civil Engineering, vol. 2018, Article ID 3780810, 10 pages, 2018. https://doi.org/10.1155/2018/3780810
Optimal Cement Mixtures Containing Mineral Admixtures under Multiple and Conflicting Criteria
Abstract
In modern construction industry, fabrication of sustainable concrete has turned the decisionmaking process into a challenging endeavor. One alternative is using fly ash and nanostructured silica as cement replacements. In these modern mixtures, proper concrete bulk density, percentage of voids, and compressive strength normally cannot be optimized individually. Hereby, a decisionmaking strategy on the replacement of those components is presented while taking into account those three performance measurements. The relationships among those components upon concrete fabrication required a design of experiments of mixtures to characterize those mineral admixtures. This approach integrates different objective functions that are in conflict and obtains the best compromise mixtures for the performance measures being considered. This optimization strategy permitted to recommend the combined use of fly ash and nanosilica to improve the concrete properties at its early age.
1. Introduction
In recent years, the environmental damages caused by the production of building materials have compelled the construction industry to seek for sustainable alternatives [1]. The partial replacement of cement by fly ash (FA), a manufacturing waste of the burning coal process, has turned into an increasingly popular alternative. Further, the addition of nanostructured SiO_{2} or nanosilica (nS) is highly recommended to counterbalance the loss of concrete compressive strength at early age caused by FA. These nanoparticles improve some valuable concrete properties such as the density, porosity, and compressive strength [2–5]. Of those properties, concrete compressive strength is the most relevant mechanical property and, therefore, the most studied [6]. Moreover, assessment of concrete porosity is necessary as this is related to concrete’s durability and permeability [7, 8]. Those characteristics depend on the number, size, and distribution of pores in the cement paste and the aggregates [9].
Hence, a range of values of the mechanical and physical properties of concrete are preferred when mineral admixtures are utilized [10, 11], as the desired characteristics depend on the proposed application. Previous works demonstrated that the specimens with higher compressive strength not necessarily corresponded to the ones with higher density and lower porosity, which are usually the desirable properties in concrete structures [12, 13]. That is why, in some cases, designers have to prioritize, for example, one characteristic over other ones. Therefore, there arises a conflict among the different performance measures of concrete. As a result, one must utilize a multiple criteria optimization method to maximize simultaneously compressive strength and density to minimize the concrete porosity. Finally, the use of this approach helps to design a multifunctional structural material by identifying the mixtures that belong to a Paretoefficient frontier [14, 15]. The resulting optimized mixtures would become the best compromise among all performance measures between the set of mixtures under evaluation.
Optimization is, therefore, a decisionmaking tool of great importance issue in the construction industry [16], where simultaneous attention is required for the environmental aspects and design factors. These frequently contradict each other especially when recycled materials (with their inherent behavioral variability) are involved.
Often, researchers have used regression models to predict performance measures, such as compressive strength, density, and porosity [17–20]. Sometimes, via neural networks, some were able to predict concrete behavior [19]. In addition, although a visual representation of the results facilitates the comparison process, other statistical methodologies can be used to compare the mixtures from a mathematical viewpoint rather than from a more subjective approach. Therefore, researchers have employed a variety of optimization approaches to find the best possible solutions in a single objective [1, 17, 21–26]. Recommendations based on all the performance measures of interest to the user are more appropriate when compared with only the selection of a single solution pertaining to the measured objective.
To address this situation, different attempts to incorporate multiple performance measures can be found [27, 28]. For instance, the constraint method, which is a formal approach to multicriteria optimization, permitted to resolve a multiobjective reliabilitybased optimum problem of prestressed concrete beams [29]. Most methods provided by the literature require target values—necessarily defined a priori—or reduce the multiobjective problem into a single objective optimization problem to find the optimal set. As a consequence, we posit a methodology that does not involve any of the previously mentioned issues that has been developed at the University of Puerto RicoMayagüez (UPRM) [13, 14, 30]. This methodology renders the Paretooptimal solution set by just defining the objectives and their respective (maximization/minimization) directions. Often, when solving a multiple criteria optimization problem, one can find a set of efficient solutions. Such a set is also known as “Paretooptimal solutions” [14, 30, 31]. These solutions are the best balances among all performance measures under evaluation; they are equally optimal since a gain in one objective results in a sacrifice in at least another objective. The optimal solutions form the Paretoefficient frontier.
In order to identify those optimal solutions, one utilizes the Paretooptimality conditions as described in Deb’s work [31]. In this work, the author stated that “A solution is said to dominate the other solution , if both the following conditions are true:(1)The solution is no worse than in all objectives. Thus, the solutions are compared based on their objective function values (or location of the corresponding points ( and ) on the objective space).(2)The solution is strictly better than in at least one objective.”
Consequently, based on the said concepts and findings, the present work focuses on the characterization of concretecontaining mineral admixtures and the subsequent multiple criteria optimization. First, a statistical design of experiments for mixtures allowed computing the mixture proportions to evaluate. Subsequently, the optimal tradeoff mixtures among compressive strength, bulk density, and percentage of voids followed. Utilizing the above conditions, we performed a full pairwise comparison between the solutions to eventually find the Paretoefficient frontier or the nondominated set. Accordingly, we present a decisionmaking strategy on the replacement of concrete components while taking into account the material’s physical and mechanical properties.
2. Experimental Methodology
2.1. Material Selection
Via a sieve analysis (ASTM 136) [32], the experimental proportions of the aggregates were determined as 30% of gravel grade #7 (ASTM C33) [33], 35% of processed aggregate (limestone), and 35% of clean sand. To determine the quantity of polycarboxylate superplasticizer (SP) necessary for each mixture, we took into account the following characteristics of the mixtures: segregation, bleeding, slump, and consistency. This minislump test was used for the mixtures at 5, 30, and 60 minutes after the mixing along with a trialanderror method to find the right proportion of superplasticizer for each mix. The evaluation criteria for slump were 100–152 mm to obtain optimun SP quantity (ASTM C143) [34].
2.1.1. Aggregates
We used gravel as coarse aggregate, with a maximum nominal size of 19.0 mm. Moreover, the processed aggregate (limestone) had a maximum nominal size of 9.5 mm. The fineness modulus of the fine aggregate was 3.0 as given in Table 1.

2.1.2. Portland Cement
We used ordinary Portland cement (OPC) Type I (ASTM C150) [35], which is classified as applicable to general purposes and have fairly high C_{3}S content for good early strength development with a specific gravity of 3.06.
2.1.3. Fly Ash
The FA class F (ASTM C618) [36] with a specific gravity of 2.38 was selected.
2.1.4. Nanosilica
Nissan Chemical Industries provided the nS used, which was opalescent and odorless amorphous silica dispersed in water, with a particle mean size of 69.40 nm and specific gravity of 2.03. The amounts of nS in the mixes are calculated based on the percentage by weight of solid in the colloidal solution. In the case of these nanoparticles, only 45% by weight is SiO_{2}. To calculate the amounts of nS for the mixtures, the amount of water and solids is considered, thus making an adjustment to the amounts of both nS and water, in order to then reach the percent established for the design. For instance, the amount of nanosilica was computed as follows: Mix design k: 9 = (PC: 0.57, FA: 0.40, and nS: 0.03) Total cementitious quantity: 672 kg/m^{3} nS (solids) = 45∗45% = 20 kg/m^{3} FA = 269 kg/m^{3} PC = 383 kg/m^{3} Sum = 672 kg/m^{3}
2.1.5. Superplasticizer
The polycarboxylate superplasticizer used followed the ASTM 494 standard [37] and was provided by a company in Puerto Rico.
2.1.6. Water
To prepare the mixtures, we employed tap water at room temperature available at the UPRM Construction Materials Laboratory.
2.2. Fabrication and Testing Procedures
A geardriven, hightorque transmission 5 L mixer (Globe SP20) manufactured by Globe Food Equipment was used to mix the concrete components. The coarse and fine aggregates were first drymixed and then placed into the mixer for 0.25 min at 120 rpm, followed by half of the required water. Then, we added the PC and later the FA (if required by the specific experiment) with the mixture working for 0.25 min at 60 rpm. The nS and SP were diluted in water in order to obtain a uniform particle distribution throughout the mixture and poured into the mixer (when used) for 4.30 min at 120 rpm. The cylindrical molds were filled by the rodding method according to ASTM C192 [38]. We removed the cylinders formwork 24 hours after casting; thereupon, we immersed them into limewater until tested at normal curing conditions (20–23°C and RH = 100%). The temperature (23–25°C) was relatively constant in the laboratory.
Following ASTM C64213 standard [39], we measured the density and percentage of voids of five specimens at 7 and 28 days of curing. We considered the specimen ovendry mass, its saturated mass after immersion in water, its saturated mass after boiling, and its immersed apparent mass. These values were used to calculate the bulk density and the volume of permeable pore space or percentage of voids of the specimens. The dimensions of the test cylinders were 76 mm in diameter and 152 mm in length to meet the minimum volume required by the standard.
For the compressive strength test, the dimensions of the test cylinders were 50 mm in diameter and 100 mm in length. We tested the compressive strength of six cylinders at 7 and 28 days of curing, using a 3000 kN Forney universal test machine according to ASTM C39 [40].
2.3. Design of Experiments
In order to generate the different combinations of the cement mixture components, that is, PC, FA, and nS [24, 41], we set up a design of experiments for mixtures. This methodology is explained in detail in our previous publication [3]. In the present work, the upper bound was set at 3% of nS and 40% of FA. In addition, the watertobinder ratio utilized for all mixtures remained constant at 0.3.
Table 2 presents the ninecomponent combinations or mixtures evaluated, as fractions of 1.00 (total mass of the mixture). Each mixture represents a solution k with different characteristics in terms of physical and mechanical properties of the resulting concrete. A multiple criteria optimization method helped us in the decisionmaking process of recommending some of these mixtures.

In this multiple criteria optimization problem, we were interested in recommending a set of alternatives (k∗) selected from the different mixture proportions of PC, FA, and nS. In view of that, the final decisionmaking would be based on the following material performance measures: compressive strength, bulk density, and percentage of voids. Naturally, the desired outcomes were higher compressive strength and density and lower percentage of voids. Thus, the strategy for the multiple criteria optimization problem is presented in Table 3.

We intended to restrict the problem described above to a manageable number of sampling experimental solutions generated through a mixture design of experiments (DOE), as mentioned previously. Furthermore, the best tradeoffs among the competing criteria were identified with the application of Paretooptimality conditions, as advocated in prior research [14, 15, 42]. This method is exact (as opposed to a heuristic approach [18]) and has being utilized previously to solve engineering and science problems [14, 15]. In this research, we applied the method to find the proportion (or fractional) combinations of a cement mixture that belong to the best possible balances in the presence of the conflicting performance measures, or more formally, the solutions in the Paretoefficient frontier.
To further demonstrate its straightforwardness, we coded the method in a commercially available spreadsheet program. Utilizing the Paretooptimality conditions, as aforementioned, we carried out a full pairwise comparison between the solutions to eventually find the Paretoefficient frontier or the nondominated set. A detailed description of the multiple criteria optimization method utilized in this work can be found in the literature [43].
3. Experimental Results
In this section, we present the experimental results organized for different curing ages. Their graphical representations have been used in the decisionmaking analysis and the optimization methodology.
3.1. Seven Days of Aging
Table 4 presents the results obtained on aging day 7. One must note that the mean compressive strength was obtained from 6 replicates, whereas the mean bulk density and average percentage of voids were from 5 replicates, due to few experimental flaws. It is apparent that if we consider each one of the performance measures separately, they will aim at different solutions (Figures 1–3). In other words, the performance measures are in conflict. Each one of the mixture combination will represent a solution or alternative k for the multiple criteria optimization problem (Table 4).

Compressive strength, bulk density, and percentage of voids are labeled f_{1}, f_{2}, and f_{3}, respectively. Then, the values of our performance measures, that is, f_{1}, f_{2}, and f_{3}, were utilized to create three matrices A_{1}, A_{2}, and A_{3} in order to compare all the solutions n in each objective.
In order to assess the first Paretooptimality condition, the following states were employed [14]:
For example, if is evaluated, the result will be −1 for the solution; 37.23 is smaller than solution 40.40 (Table 5). In this context, smaller means better because we are trying to minimize each performance measurement. Then, one can perform the same comparison in each objective for all its solutions (Table 6 and 7).



Now, matrix S is constructed to compare all the objectives and evaluate the second Paretooptimality condition (Table 8). By this means, one can identify the nondominated solution set using the following conditions:

Finally, when we sum each row of matrix S, we can identify the solutions that are part of the Paretoefficient frontier, that is, the sum associated with that row (solution) is less than 3000 (in this case).
After applying the multiple criteria optimization method, Table 9 shows in bold the efficient solutions for aging day 7. These were the mixtures numbered 2, 8, and 9. Mixture number 2 is the control mixture with only Portland cement (no replacement). We expected that this mixture be in the optimal set since its properties were very competitive during its early age. However, we found particularly interesting that the other two mixtures, that is, 8 and 9, that belong to the Paretoefficient frontier contained FA and nS. Mixture 8 had 78.5% PC, 20% FA, and 1.5% nS, while mixture 9 possessed 57% PC, 40% FA, and 3% nS. Although mixture 9 had 40% of FA (high level of replacement), the addition of only 3% nS makes it a competitive combination with adequate physical and mechanical properties. In contrast, mixture 3 is made of 60% PC, 40% FA, and no nanoparticles (0% nS), which has a high level of replacement; notwithstanding, this mixture does not belong to the Paretoefficient frontier. Intriguingly, mixture 1 (20% FA and no nS) had a similar behavior. Hence, the difference between being and not being part of the Paretoefficient frontier appeared to be the presence of the silica nanoparticles. This was a consequential finding that is discussed later.

As we analyzed three performance measures, the results yielded the 3D graph in Figure 4. In addition, one can employ a cone of Pareto dominance to visualize the dominated and nondominated solutions. Figure 4 shows all the solutions k (mixtures) in the criteria space with a rotated view to make easier the visualization of the efficient frontier.
3.2. TwentyEight Days of Aging
Table 10 shows the average results of the three performance measures evaluated at 28 days of aging. Clearly, mixture 8 had a higher compressive strength, whereas mixture 6 bears a larger bulk density and lower percentage of voids. This leads, once again, to a conflict between the objectives.

As in the analysis of day 7, at day 28, we sought to maximize the compressive strength and bulk density and to minimize the percentage of voids. Table 11 presents the results obtained from the multiple criteria optimization strategy, which indicates that four solutions belong to the Paretoefficient frontier: mixtures 2, 6, 7, and 8. The Paretooptimality conditions can be used to ensure that these sets of mixtures are always better in at least one objective and the same or worse in the other objective.

We did expect mixture number 2 to be part of the Paretoefficient frontier since it is the control mixture with only PC. Mixtures 6 and 7 contain PC and 1.5% and 3.0% nS, respectively, without any FA, that is, one of the replacements of interest. Conversely, mixture 8, which contains 20% FA (with 78.5% PC and 1.5% nS), is also efficient. The solutions can be observed in the criteria space in Figure 5 with a rotated view for visualization convenience.
4. Discussion of Results
The results obtained from the multiple criteria optimization are the best tradeoff mixtures recommended to the decisionmakers who can then select a single mixture among the efficient set presented in this work. Naturally, such a decision should be based on the characteristics of the mixtures presented in each performance measures. Also, they should consider the proportion of each component in the mixture. This depends on the user’s (or structural designer’s) interest about the mineral admixtures and the specific application of each concrete mixture.
The optimization process revealed that mixtures with FA and no nS did not belong to the Paretoefficient frontier. This behavior was observed throughout the analysis, denoting that the addition of silica nanoparticles is necessary when FA is presented as cement replacement. This beneficial interaction had already been observed in prior works [4]. In such concretes, the nanoparticles do improve the physical and mechanical properties of the resulting concrete. Toutanji et al. [44] discovered that a combination of different supplementary materials, as silica fume, increased the compressive strength. Previous works support these findings [17], where the use of FA and nS was found to improve the concrete microstructure and rate of strength gain. Microstructure analysis of concrete by scanning, scanning transmission, and transmission electron microscopy revealed that nS particles fill the CSHgel structure voids and act as nuclei, tightly bonded with the CSH particles [45]. This tight packing densifies concrete, protecting it from chemical attacks and leaching, while enhancing its durability and mechanical properties.
As aforementioned, after seven days of aging, there were three efficient mixtures. In the analysis at day 28, the efficient mixtures were four. Examining this pool of efficient mixtures reveals that two were efficient in all the analysis conducted: (a) the control mixture with 100% PC, 0% FA, and 0% nS and (b) the mixture with 78.5% PC, 20% FA, and 1.5% nS. In other words, for the two ages tested, the regular mix (control) can be replaced by mixture 8, which even has higher compression strength at the expense of a slight increase in porosity. This result further proves how nanosilica can counteract some strength loss induced by the FA presence [2, 5, 17, 46]. This is an important finding as it points to the formulation of a sustainable concrete, that is, one that requires less cement to attain structural behavior, using an industrial waste, that is, fly ash and nanostructured SiO_{2} particles. In effect, less consumption of cement would lead to a smaller carbon footprint upon its fabrication, without compromising the structural strength of the mixture.
However, the cost of large amounts of nS, as a construction project would demand, poses an economic challenge. On the other hand, FA is one of the lowpriced mineral admixtures, which could balance the final cost of concrete. Therefore, to finally propose the use of nS and FA in structural concrete, we deem critical to an optimization strategy that includes an exhaustive cost analysis.
Finally, the full pairwise comparison between solutions that led us to the Paretoefficient frontier was implemented in a readily available spreadsheet package. This means that no computational intricacy was required to render a robust analysis of the data to assist in the decisionmaking process. We recognize that the multiple criteria optimization method, in our case, studied only three material characteristics, that is, compressive strength, density, and void presence. Concrete is a versatile material with numerous potential variables arising from its fabrication process. Nonetheless, the multiple criteria optimization method is a versatile and scalable strategy that could be expanded to include other performance measures more relevant to other specific applications of concrete mixtures.
5. Conclusions
The present work proposes the use of an optimization procedure to determine for nanosilicacontaining concrete mixtures the best ones to achieve specific performance measures: concrete compressive strength, bulk density, and percentage of voids (porosity). These performance measurements were measured after 7 and 28 days. The nine proportion combinations evaluated contained different percentages of PC, FA, and nS. The use of the multiple criteria optimization helped find the mixtures that were the best balances among the studied objectives. At day 7, three mixtures were part of the Paretoefficient frontier. Two of them were mixtures with cement replacement, that is, FA and nS at different levels. On the other hand, four mixtures were part of the Paretoefficient frontier at day 28. This time, one mixture has cement replacement (FA and nS). In addition, two mixtures were efficient at either day 7 or day 28.
As a consequence, the multiple criteria optimization strategy permitted to recommend the use of FA and nS to improve the concrete properties. However, if the analysis is performed considering only one performance measurement, such as compressive strength, the option of cement replacement by FA is not recommended. Hence, taking into consideration several performance measurements, the use of mineral admixtures is suggested. This is because a mixture with mineral admixtures will be equally optimal than a control mixture with just PC when more properties are considered. Consequently, as the decisionmakers know the best tradeoff mixtures for an individual application, the final recommendation is easier to make.
Conflicts of Interest
The authors declare that they have no conflicts of interest.
Acknowledgments
This material is based upon the work supported by the National Science Foundation under Grants nos. HRD 0833112 and 1345156 (CREST program). Additional support was provided by the US Department of Education through Grant no. P120A120097 (MSEIP program). The authors would like to thank the technical personnel of the Nanotechnology Center and the Construction Materials Laboratory of the University of Puerto Rico for their invaluable assistance in the completion of this work.
References
 J. OliverSola, A. Josa, J. Rieradevall, and X. Gabarrell, “Environmental optimization of concrete sidewalks in urban areas,” International Journal of Life Cycle Assessment, vol. 14, no. 4, pp. 302–312, 2009. View at: Publisher Site  Google Scholar
 L. E. Zapata, G. Portela, O. M. Suárez, and O. Carrasquillo, “Rheological performance and compressive strength of superplasticized cementitious mixtures with micro/nanoSiO_{2} additions,” Construction and Building Materials, vol. 41, pp. 708–716, 2013. View at: Publisher Site  Google Scholar
 N. M. García, L. E. Zapata, O. M. Suárez, and M. CabreraRíos, “Effect of fly ash and nanosilica on compressive strength of concrete at early age,” Advances in Applied Ceramics, vol. 114, no. 2, pp. 99–106, 2015. View at: Publisher Site  Google Scholar
 L. E. ZapataOrduz, G. Portela, and O. M. Suárez, “Tensile behavior by Weibull analysis in binary, ternary, and quaternary concretes designed with micro and nanosilica additions,” in Maintenance, Monitoring, Safety, Risk and Resilience of Bridges and Bridge Networks, pp. 1254–1261, CRC Press, Boca Raton, FL, USA, 2016. View at: Google Scholar
 L. E. ZapataOrdúz, G. Portela, and O. M. Suárez, “Weibull statistical analysis of splitting tensile strength of concretes containing class F fly ash, micro/nanoSiO_{2},” Ceramics International, vol. 40, no. 5, pp. 7373–7388, 2014. View at: Publisher Site  Google Scholar
 G. Shakhmenko, I. Juhnevica, and A. Korjakins, “Influence of solgel nanosilica on hardening processes and physicallymechanical properties of cement paste,” Procedia Engineering, vol. 57, pp. 1013–1021, 2013. View at: Publisher Site  Google Scholar
 J. G. Cabrera, P. A. Claisse, and D. N. Hunt, “Measurement of porosity as a predictor of the durability performance of concrete with and without condensed silica fume,” Advances in Cement Research, vol. 13, no. 4, pp. 165–174, 2001. View at: Publisher Site  Google Scholar
 L. Basheer, J. Kropp, and D. J. Cleland, “Assessment of the durability of concrete from its permeation properties: a review,” Construction and Building Materials, vol. 15, no. 23, pp. 93–103, 2001. View at: Publisher Site  Google Scholar
 C. Lian, Y. Zhuge, and S. Beecham, “The relationship between porosity and strength for porous concrete,” Construction and Building Materials, vol. 25, no. 11, pp. 4294–4298, 2011. View at: Publisher Site  Google Scholar
 I. Kaur and R. Siddique, Mechanical Properties of High Volume Fly Ash (HVFA) Concrete Subjected to Elevated Temperatures up to 120°C, Thapar Institute of Engineering & Technology University, Patiala, India, 2005, M.E. thesis.
 P. Lawrence, M. Cyr, and E. Ringot, “Mineral admixtures in mortars effect of type, amount and fineness of fine constituents on compressive strength,” Cement and Concrete Research, vol. 35, no. 6, pp. 1092–1105, 2005. View at: Publisher Site  Google Scholar
 J. Sunku, “Advantages of using fly ash as supplementary cementing material (SCM) in fibre cement sheets,” in Proceedings of 10th International Inorganicbonded Fiber Composites Conference, pp. 25–32, São Paulo, Brazil, November 2006. View at: Google Scholar
 R. S. Ravindrarajah, “Bleeding of fresh concrete containing cement supplementary materials,” in Proceedings of 9th East AsiaPacific Conference on Structural Engineering and Construction, pp. 16–18, Bali, Indonesia, December 2003. View at: Google Scholar
 C. J. Burgos, J. M. Pizarro, K. I. CamachoCáceres, and M CabreraRíos, “A visual basic tool for multiple criteria optimization,” in Proceedings of the 2014 Industrial and Systems Engineering Research Conference, Montreal, Canada, November 2014. View at: Google Scholar
 B. RodríguezYañez, Y. M. MéndezVázquez, and M. CabreraRíos, “Simulationbased process windows simultaneously considering two and three conflicting criteria in injection molding,” Production & Manufacturing Research, vol. 2, no. 1, pp. 603–623, 2014. View at: Publisher Site  Google Scholar
 D. JatoEspino, E. CastilloLopez, J. RodriguezHernandez, and J. C. CanterasJordana, “A review of application of multicriteria decision making methods in construction,” Automation in Construction, vol. 45, pp. 151–162, 2014. View at: Publisher Site  Google Scholar
 L. E. Zapata Orduz, Rheological and Mechanical Characterization of Portland Cement Mixes Containing Micro and Nano Amorphous Silica Particles, University of Puerto Rico, Mayaguez, PR, USA, 2013, Ph.D. dissertation.
 A. Baykasoğlu, A. Öztaş, and E. Özbay, “Prediction and multiobjective optimization of highstrength concrete parameters via soft computing approaches,” Expert Systems with Applications, vol. 36, no. 3, pp. 6145–6155, 2009. View at: Publisher Site  Google Scholar
 K. S. Kulkarni, S. C. Yaragal, and K. S. Babu Narayan, “An overview of high performance concrete at elevated temperatures,” International Journal of Applied Engineering and Technology, vol. 1, pp. 48–60, 2011. View at: Google Scholar
 E. Ghafari, H. Costa, E. Júlio, A. Portugal, and L. Durães, “The effect of nanosilica addition on flowability, strength and transport properties of ultra high performance concrete,” Materials & Design, vol. 59, pp. 1–9, 2014. View at: Publisher Site  Google Scholar
 M. A. Hassanain and R. E. Loov, “Cost optimization of concrete bridge infrastructure,” Canadian Journal of Civil Engineering, vol. 30, no. 5, pp. 841–849, 2003. View at: Publisher Site  Google Scholar
 C. Perea, I. Payá, V. Yepes, and F. González, “Heuristic optimization of reinforced concrete building frames,” in Proceedings of the 2nd International FIB Congress, p. 9, Naples, Italy, June 2006. View at: Google Scholar
 M. AnsonCartwright, Optimization of Aggregate Gradation Combinations to Improve Concrete Sustainability, University of Toronto, Toronto, ON, Canada, 2011, M.S. Thesis.
 O. Akalin, K. U. Akay, B. Sennaroglu, and M. Tez, “Optimization of chemical admixture for concrete on mortar performance tests using mixture experiments,” Chemometrics and Intelligent Laboratory Systems, vol. 104, no. 2, pp. 233–242, 2010. View at: Publisher Site  Google Scholar
 E. M. R. Fairbairn, M. M. Silvoso, R. D. Toledo Filho, J. L. D. Alves, and N. F. F. Ebecken, “Optimization of mass concrete construction using genetic algorithms,” Computers & Structures, vol. 82, no. 23, pp. 281–299, 2004. View at: Publisher Site  Google Scholar
 A. Rudy and J. Olek, “Optimization of mixture proportions for concrete pavements—influence of supplementary cementitious materials, paste content and aggregate gradation, joint transportation research program,” Tech. Rep. FHWA/IN/JTRP2012/34, Indiana Department of Transportation and Purdue University, West Lafayette, IN, USA, 2012. View at: Google Scholar
 B. Şimşek, Y. T. İç, and E. H. Şimşek, “A TOPSISbased Taguchi optimization to determine optimal mixture proportions of the high strength selfcompacting concrete,” Chemometrics and Intelligent Laboratory Systems, vol. 125, pp. 18–32, 2013. View at: Publisher Site  Google Scholar
 M. F. Ghazy and M. F. A. El Hameed, “Optimization of lightweight concrete process by GrayTaguchi method,” ACI Materials Journal, vol. 112, no. 3, pp. 365–374, 2014. View at: Publisher Site  Google Scholar
 S. Barakat, K. BaniHani, and M. Q. Taha, “Multiobjective reliabilitybased optimization of prestressed concrete beams,” Structural Safety, vol. 26, no. 3, pp. 311–342, 2004. View at: Publisher Site  Google Scholar
 X. K. Zou, C. M. Chan, G. Li, and Q. Wang, “Multiobjective optimization for performancebased design of reinforced concrete frames,” Journal of Structural Engineering, vol. 133, no. 10, pp. 1462–1474, 2007. View at: Publisher Site  Google Scholar
 K. Deb, MultiObjective Evolutionary Optimisation for Product Design and Manufacturing, L. Wang, A. Ng, and K. Deb, Eds., Springer, London, UK, 2011.
 ASTM Standard C136, Standard Test Method for Sieve Analysis of Fine and Coarse Aggregates, vol. 14, ASTM International, West Conshohocken, PA, USA, 2001.
 ASTM Standard C33, Standard Specification for Concrete Aggregates, ASTM International, West Conshohocken, PA, USA, 2003.
 ASTM Standard C143, Standard Test Method for Slump of HydraulicCement Concrete, ASTM International, West Conshohocken, PA, USA, 2005.
 ASTM Standard C150/C150M12, Standard Specification for Portland Cement, ASTM International, West Conshohocken, PA, USA, 2012.
 ASTM Standard C61812a, Standard Specification for Coal Fly Ash and Raw or Calcined Natural Pozzolan for Use in Concrete, ASTM International, West Conshohocken, PA, USA, 2012.
 ASTM Standard C494/C494M13, Standard Specification for Chemical Admixtures for Concrete, ASTM International, West Conshohocken, PA, USA, 2013.
 ASTM Standard C192/C192M−13a, Standard Practice for Making and Curing Concrete Test Specimens in the Laboratory, ASTM International, West Conshohocken, PA, USA, 2013.
 ASTM Standard C642, Standard Test Method for Density, Absorption, and Voids in Hardened Concrete, ASTM International, West Conshohocken, PA, USA, 2013.
 ASTM Standard C39, Standard Test Method for Compressive Strength of Cylindrical Concrete Specimens, ASTM International, West Conshohocken, PA, USA, 2004.
 R. H. Myers and D. Montgomery, Response Surface Methodology, John Wiley and Sons, Danvers, MA, USA, 2002.
 M. L. SánchezPeña, C. E. Isaza, J. PérezMorales, C. RodríguezPadilla, J. M. Castro, and M. CabreraRíos, “Identification of potential biomarkers from microarray experiments using multiple criteria optimization,” Cancer Medicine, vol. 2, no. 2, pp. 253–265, 2013. View at: Publisher Site  Google Scholar
 K. I. Camacho, OptimizationDriven MetaAnalysis: The Simultaneous Search for Cancer Biomarkers with Multiple Microarray Experiments, University of Puerto Rico, Mayagüez, PR, USA, 2014, M.S. thesis.
 H. Toutanji, N. Delatte, S. Aggoun, R. Duval, and A. Danson, “Effect of supplementary cementitious materials on the compressive strength and durability of shortterm cured concrete,” Cement and Concrete Research, vol. 34, no. 2, pp. 311–319, 2004. View at: Publisher Site  Google Scholar
 G. Quercia and H. J. H. Brouwers, “Application of nanosilica (nS) in concrete mixtures,” in Proceedings of 8th fib International Ph.D. Symposium in Civil Engineering, pp. 1–6, Kongens Lyngby, Denmark, June 2010. View at: Google Scholar
 L. E. Zapata Orduz, G. Portela, O. M. Suárez, and A. D. Cáceres, “Compatibility analysis between Portland cement type I and micro/nanoSiO_{2} in the presence of polycarboxylatetype superplasticizers,” Cogent Engineering, vol. 3, no. 1, pp. 1–18, 2016. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2018 Nitza M. García et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.